The Alloy-Theoretic Automated Toolkit (ATAT):A User Guide

Axel van de Walle

August 13,2013

2

Chapter 1

Introduction

The Alloy-Theoretic Automated Toolkit (ATAT) is a generic name that refers to a collection of alloy theory

tools:

• A code to construct cluster expansions from ﬁrst-principles (MAPS).A cluster expansion is a very

compact and eﬃcient expression giving the energy of an substitutional alloy as a function of its con-

ﬁguration (i.e.which type of atom sits where on the lattice).

• A code to perform Monte Carlo simulation of lattice models in order to compute thermodynamic

properties of alloys starting from a cluster expansion.

• Extension of the two above tools that allow the construction of so-called reciprocal-space cluster ex-

pansion,which are useful to model the energetics of alloys exhibiting a large atomic size mismatch.

• Utilities to interface the above tools with ﬁrst-principles codes (such as VASP).

• Job control utilities that enable the eﬃcient use of a cluster of workstations to run the ﬁrst-principles

codes that provide the input to the above codes.

3

4 CHAPTER 1.INTRODUCTION

Chapter 2

Credits and Licence

The Alloy-Theoretic Automated Toolkit (ATAT)

1

is a generic name that refers to a collection of alloy theory

tools developped by Axel van de Walle

2

,in collaboration with various research groups.

2.1 Collaborators

The MAPS

3

(MIT Ab-initio Phase Stability) code,which automatically constructs a cluster expansion

from the result of ﬁrst-principles calculations,was developped by Axel van de Walle in collaboration with

Prof.Gerd Ceder’s group

4

from the Department of Materials Science and Engineering at the Massachusetts

Institute of Technology.MAPS consists of the following codes:maps,corrdump,genstr,checkcell,kmesh,

cv.

The EMC2 (Easy Monte Carlo Code),which automate the calculation of alloy thermodynamic properties

via Monte Carlo simulations of lattice models,were developped by Axel van de Walle in collaboration with

Prof.Mark Asta’s group

5

from the Department of Materials Science and Engineering at Northwestern

University.EMC2 consists of the following codes:emc2,phb.

The CSE (Constituent Strain Extension) to both the MAPS and EMC2 codes,which implement the

constituent strain formalism based on a reciprocal-space cluster expansion,was developped by Axel van de

Walle in collaboration with Alex Zunger’s Solid State Theory Group

6

at the National Renewable Energy

Laboratory in Golden,Colorado and in collaboration with Gus Hart

7

from the Department of Physics and

Astronomy at Northern Arizona University.CSE conssists of the following ﬁles:csﬁt.cc predcs.cc,predrs.cc,

kspacecs.cc.

Mayeul D’Avezac at NREL has provided all the changes needed for ATAT to compile with g++ versions

4.1 and later as well as intel’s c++ compiler.

Volker Blum at NREL has contributed to improve the portability of the package by providing a perl

version of the chl utility.

Dongwon Shin at Penn State has converted a large number of common lattices (found at the NRL navy

web site

8

) into the atat format.See directory data/str.

Greg Pomrehn has improved the eﬃciency of the structure enumeration algorithm and contributed the

script mmapsrep.

The FFT routines in the ﬁles ﬀtn.cc and ﬀtn.h were obtained from the NIST Guide to Available Math

Software (GAMS).The origin of these routines dates back to a FORTRAN code by R.C.Singleton in 1968,

later converted to C and subsequently improved by Mark Olesen and John Beale in 1995.These routines are

1

http://www.its.caltech.edu/˜avdw/atat/

2

http://www.mit.edu/˜avdw/

3

http://www.mit.edu/˜avdw/maps

4

http://burgaz.mit.edu/

5

http://cms.northwestern.edu/

6

http://www.sst.nrel.gov/

7

http://www.phy.nau.edu/˜hart/

8

http://cst-www.nrl.navy.mil/lattice/

5

6 CHAPTER 2.CREDITS AND LICENCE

included in the atat package for sole purpose of providing users with the convenience of avoiding a separate

download.Axel van de Walle does not claim any ownership of them or intellectual credit for them.

Gao Zhe has contributed an interface to PWSCF (aka QuantumEspresso) that can be found in atat/glue/qe

Matt Probert has contributed an interface to CASTEP that can be found in atat/glue/castep/

2.2 Financial Support

The development of MAPS was supported by the U.S.Department of Energy,Oﬃce of Basic Energy Sciences,

under contract no.DE-F502-96ER 45571.Gerbrand Ceder acknowledges support of Union Mini`ere through

a Faculty Development Chair.Axel van de Walle acknowledges support of the National Science Foundation

under program DMR-0080766 and DMR-0076097 during his stay at Northwestern University.

The development of EMC2 was supported by the NSF under program DMR-0080766.

The development of the CSE is supported by the NSF under program DMR-0080766.

The development of the tensorial cluster expansion (GCE and gencs code) is supported by the Center

for the Science and Engineering of Materials at Caltech,an NSF-funded MRSEC and by the NSF CMMT

grant DMR-0907669.

The development of the wycked and getproto codes is supported by the NSF CAREER grant DMR-

1154895.

The development of the mcsqs code is supported by ONRgrants N00014-11-1-0886 and N00014-11-1-0886.

2.3 Licence and Agreements

Any scientiﬁc article or book whose results were obtained with the codes described above must properly

acknowledge their use by citing the following papers:

1.A.van de Walle and G.Ceder,“Automating First-Principles Phase Diagram Calculations

9

”,Journal

of Phase Equilibria,23,348,(2002).

2.A.van de Walle and M.Asta,“Self-driven lattice-model Monte Carlo simulations of alloy thermody-

namic properties and phase diagrams

10

”,Modelling Simul.Mater.Sci.Eng.10,521,(2002).

3.A.van de Walle,M.Asta and G.Ceder,“The Alloy Theoretic Automated Toolkit:AUser Guide

11

”CALPHAD

Journal,26,539,(2002).

4.A.van de Walle,“Multicomponent multisublattice alloys,nonconﬁgurational entropy and other addi-

tions to the Alloy Theoretic Automated Toolkit

12

”,Calphad Journal 33,266,(2009).

5.As of version 2.81,the algorithm to generate superstructures has been improved based on the ideas in

G.L.W.Hart and R.W.Forcade,“Algorithm for generating derivative structures

13

,” Phys.Rev.B

77,224115,(2008).

6.If the mcsqs code is used:A.van de Walle and P.Tiwary and M.M.de Jong and D.L.Olmsted and

M.D.Asta and A.Dick and D.Shin and Y.Wang and L.-Q.Chen and Z.-K.Liu,Eﬃcient stochastic

generation of Special Quasirandom Structures

14

,Calphad Journal 42,13 (2013).

7.If the constituent strain extension is used:D.B.Laks and L.G.Ferreira and S.Froyen and A.Zunger,

Phys.Rev.B 46,p.12587 (1992).

8.The wycked code uses the Wyckoﬀ position database from the Bilbao Crystallographic Server

15

.Ac-

cordingly,if you use this code,you should also cite the following papers:

9

http://arXiv.org/abs/cond-mat/0201511

10

http://arXiv.org/abs/cond-mat/0201473

11

http://arxiv.org/abs/cond-mat/0212159

12

http://arxiv.org/abs/0906.1608

13

http://link.aps.org/abstract/PRB/v77/e224115

14

http://dx.doi.org/10.1016/j.calphad.2013.06.006

15

http://www.cryst.ehu.es/

2.4.BETA TESTERS 7

M.I.Aroyo,J.M.Perez-Mato,D.Orobengoa,E.Tasci,G.de la Flor,A.Kirov,“Crystallography

online:Bilbao Crystallographic Server”,Bulg.Chem.Commun.43 183 (2011).

M.I.Aroyo,J.M.Perez-Mato,C.Capillas,E.Kroumova,S.Ivantchev,G.Madariaga,A.Kirov

and H.Wondratschek,“Bilbao Crystallographic Server I:Databases and crystallographic com-

puting programs”,Z.Krist.221,15 (2006).

M.I.Aroyo,A.Kirov,C.Capillas,J.M.Perez-Mato and H.Wondratschek,“Bilbao Crystallo-

graphic Server II:Representations of crystallographic point groups and space groups”,Acta Cryst.

A62,115 (2006).

9.The getproto code uses processed data from the index of the Landolt-Bornstein database

16

.This

data is available upon request by contacting avdw@alum.mit.edu

17

if you can show that you have

access to this database.Also,if using this data,please cite:Villars,P.,Cenzual,K.,Daams,J.,

Gladyshevskii,R.,Shcherban,O.,Dubenskyy,V.,Melnichenko-Koblyuk,N.,Pavlyuk,O.,Stoiko,

S.,Sysa,L.,“Landolt-Brnstein — Group III Condensed Matter:Numerical Data and Functional

Relationships in Science and Technology”,Edited by Villars,P.and Cenzual,K.,SpringerMaterials —

The Landolt-Brnstein Database,Volume 43A1-43A10 (2013).

The ﬁles included in this distribution cannot be further distributed either in their original or in a modiﬁed

form without consent of the author,Axel van de Walle (avdw@alum.mit.edu).

Users are free to modify the code solely for their personal use and are encouraged to share their improve-

ments with the author at (avdw@alum.mit.edu

18

).Their contributions will be acknowledged in the present

section,in future versions of this manual.

2.4 Beta testers

The following researchers have provided numerous constructive comments that have proven extremely useful

to improve the quality of the program.

1.Dane Morgan (University of Wisconsin)

2.Paul Dalach (Northwestern)

3.Dinesh Balachandran (MIT,Gerd Ceder’s group)

4.Ben Burton (National Institute of Standards and Technology)

5.Gautam Ghosh (Northwestern University)

6.Nikolai Andreevich Zarkevich (University of Illinois at Urbana-Champaign,Duane Johson’s group)

7.Volker Blum (NREL,Alex Zunger’s group)

8.Chris Woodward (Northwestern University/Air Force)

9.Zhe Liu (Northwestern University,Mark Asta’s group)

10.Yi Wang and Raymundo Arroyave (Pennsylvania State University,Long-Qing Chen and Zi-Kui Liu’s

group)

11.Elif Ertekin (University of California at Berkeley,Daryl Chrzan’s group)

12.Rodrigo Barbosa Capaz (University of California at Berkeley)

13.Sundar Amancherla (General Electric)

16

http://www.springermaterials.com/

17

mailto:avdw@alum.mit.edu

18

mailto:avdw@alum.mit.edu

8 CHAPTER 2.CREDITS AND LICENCE

Chapter 3

Getting started

3.0.1 Requirements

You need the following utilities installed:

• g++ version 2.7.2 or later.Type g++ --version to verify this.This package can be downloaded from

http://www.gnu.org/.

• GNU make (any version).Type make --version to verify this.On some systems this command may

be called gmake or gnumake.This package can be downloaded from http://www.gnu.org/.

• A ﬁrst-principle electronic structure calculation code,such as VASP

1

• You may want to use gnuplot to plot the output of the code.Type gnuplot and check the program

starts (Type q to quit).If not,it can be downloaded from http://www.gnuplot.info/.

• You may need ssh if you have multiple machines and they are connnected through an unsecure network

(e.g.the internet).This package can be downloaded from http://www.openssh.com/.

3.0.2 Installation

If you have an earlier version of ATAT installed,please delete or rename the former atat directory before

proceeding,e.g.,

mv atat atatold

Then,type

gunzip atatX

XX.tar.gz

tar -xvf atatX

XX.tar.gz

where X

XX is the current version number.These commands create a directory called atat in the current

directory.It contains the whole package.For future reference,I’ll call the whole access path to this directory

atat.

Type

cd atat

and open the ﬁle makefile with a text editor and look for the line BINDIR=$(HOME)/bin/.Change

$(HOME)/bin/to point wherever you want to put the executables.Type

make

If no error message appears,proceed with the next steps,otherwise consult Chapter 8.

make install

rehash (not necessary with bash shell)

1

http://cms.mpi.univie.ac.at/vasp/

9

10 CHAPTER 3.GETTING STARTED

3.0.3 Test MAPS with a simple example

Change to a directory of your choice (preferably empty) and type

cp atat/examples/cuau.in lat.in

maps -d &

Maps is running and waiting for a signal.Type

touch ready

to indicate that you are ready to for maps to generate a structure.Maps replies Finding best structure...

To ﬁnd the structure just created,wait for done to appear and type:

ls */wait

to observe that directory 0 has been created.This directory contains a ﬁle str.out which describes the

structure whose energy needs to be calculated.The ﬁle wait is just a ﬂag that allows you to ﬁnd the newly

created directory.Let’s pretend that we have computed the energy of that structure.We need to let maps

know about it.Type,for instance:

echo 1.1 > 0/energy (If 1.1 is the energy of the structure.)

rm 0/wait

Maps responds by Finding best cluster expansion...,followed by done.You can repeat the process

(touch ready,etc.) to add more structures.Maps will update the current cluster expansion every time a

new energy becomes known.(By default,maps checks every 10 sec.).For a description of the output ﬁles,

type:

maps -h | more

or refer to section 7 A nice utility called mapsrep allows you to plot the results using gnuplot.To stop maps

cleanly,type:touch stop

Suggestion:to clarify the output of the program,it is recommended that you run maps in one terminal

window and type all other command in another terminal window.

3.1 Install the interface between MAPS and VASP

Type

ezvasp

and follow the instructions posted on the screen to conﬁgure this command.

To test this interface,change to a directory of your choice and type

maps -d &

(unless maps is running already in that same directory).

While MAPS automatically create ﬁles that describe the geometry of the structures (calledn/str.out,

where n is the structure name),we need to provide a ﬁle containing all the other parameters needed by the

ﬁrst-principles code.Type:

cp atat/glue/vasp/vasp.wrap.

to copy an example of such ﬁle in the current directory.For a description of these parameters,type:

ezvasp -h | more

Let’s say you have a new structure in directory 0 (created by typing touch ready).Type:

3.2.INSTALL AND TEST THE JOB CONTROL UTILITIES 11

cd 0

runstruct

vasp

When the command has terminated,the directory 0 will contain a ﬁle energy giving the energy of the

structure.If error messages appear consult Chapter 8.

If no error messages appear,you can proceed another level up in automation.Type

cd..(to go back into the main directory)

pollmach runstruct

vasp &

This script will automatically call the above command repeatedly.To stop it cleanly,type:

touch stoppoll

(Disregard the warning message.) If you only have access to one machine,this is as good as it gets,if you

have more than one machine,read the next section.If you want to use another code than VASP,read section

3.3.

3.2 Install and test the job control utilities

This section requires some knowledge of UNIX,but it is worth it!Networking problems can be tricky and we

will test various thing as we go along.You only need to perform this installation on your ”master” machine

that will run maps.All other machine (which we be called the “remote” machines) only need to have VASP

(or any other ab-initio code).

Before you start,you must ﬁrst make sure that it is possible to login from the master machine to the

remote machines without entering a password.This is essential for the program to be able to run on its

own,without your intervention.Don’t worry it is generally possible to do this without compromising the

security of your system.Two commands allow you to run a command on a remote machine.If the master

and remote machines are connected through a secure network (e.g.a beowolf cluster having its own local

network) or if you don’t care about security (for now),you can use rsh.Otherwise,ssh provides a secure

way to command a machine remotely.

To set up rsh so that you can login without typing a password,you must have the appropriate.rhosts

ﬁle on the remote machine.For more information,consult the rsh man page.(One important issue,often

not mentioned in the man pages,its that you need to set the ﬁle permissions of the.rhosts ﬁle so that

noone else but you has “write” permission:chmod og-w ~/.rhosts).

To set up ssh so that you can login without typing a password,consult the ssh man page,especially

the section on “RSA-based host authentication”.(This is the feature that makes the login secure even if no

password is needed.) In general,setting this up involves creating a.shosts ﬁle and generating a public key

ﬁles to be copied onto the remote machines.

If your username is diﬀerent on the remote machine and if you use ssh,use the syntax node username@host

instead.If you use rsh,use the syntax node -l username host.

Once you are able to run either rsh node2 ls or ssh node2 ls and get the content of your home

directory on the remote machine (assuming that you have a remote machine called node2),you can proceed

to the next step.Do you have the same home directory on the master and remote machines and does it have

the same access path?To check this,cd to some arbitrary subdirectory and type:

node node2 ls

where node is a command provided with ATAT and node2 is the name of the remote machine.If you want

to use ssh instead,type

node -s node2 ls

This should print the content of the current directory on the master machine (not your home directory).If

you get an error message or if you get the content of another directory,you will need to check if the following

works.Make sure you are in a directory that does not contain too many ﬁles.If you want to use rsh,type:

12 CHAPTER 3.GETTING STARTED

node -r node2 ls

while if you want to use ssh

node -s -r node2 ls

In either case,you should get the content of the current directory before continuing on.The node -r

command works by copying the content of the current directory on the remote machine in a temporary

directory.Once the command has terminated,the new content is copied back and the remote temporary

directory is deleted.

We are now ready to automate the calculations.Type

chl

and,as indicated on the screen,open the ﬁle ~/.machines.rc with a text editor.This ﬁle contains numerous

comment lines explaining the format of the ﬁle and a few examples.

The commands in the ﬁrst column (before the +) must print a single number indicating the load of the

machine.It is a good check to copy and paste each of these command,one at the time,into a shell window

to see if the output is a single number.In order to extract a single number out of a complicated output,the

command getvalue is provided.It extracts the single number following the token given as an argument.

The ﬁrst entry,with the none keyword after the + indicates the threshold load above which a machine is

considered too busy to be usable.Note that the load checking commands may quite elaborate if,for instance,

you need to “rescale” the load of some machines because they have a diﬀerent reporting scheme or if you

want to tweak the priority given to each machine.

The second column (after the +) give the command preﬁx needed to run on each remote machine.These

preﬁx will usually consist of the command node described above.It is very important that the command

preﬁx be such that the current directory in the remote machine when the command is run is the same as on

the local machine.The best way to test that is to try the preﬁx in front of the ls command and verify that

what is printed is indeed the content of the current local directory.

Once you are done with entering the information for each of your machines (you can also enter only

a few and come back later to add the remaining ones),make sure to comment out the examples provided

(placing a#at the beginning of the unwanted line).Do not comment out the ﬁrst line which contains the

none keyword.

Once you have edited the ~/.machines.rc ﬁle,type chl.This should give a list of the load of all

machines in the ﬁrst column and a list of command preﬁx in the second.Next,try the command minload.

It should give the command preﬁx that let you access the machine with the minimum load or none if no

machine is available.To check,once again,that the command preﬁx are correct,type ‘minload‘ ls (make

sure you use backward quotes!).This should print the content of the current directory (unless there are no

machines available).

3.3 Interfacing MAPS with other ﬁrst-principles codes

You need to provide a command (e.g.a shell script) called runstruct

xxx,where xxx is any name of your

choice.This script should read,from the current directory,the ﬁle str.out describing the geometry of

the structure and create the appropriate input ﬁles for the ﬁrst-principles code.It should then execute the

command(s) needed to run the code.If a multiple machine environment is used,the script should use the

ﬁrst argument passed to the script ($1) as command preﬁx to put in front of any command in order for them

to be run on a remote machine.That is,if the ﬁrst-principle code is called ”myfp” the script should execute

$1 myfp

Once the ﬁrst-principles code has terminated,the script should

• Create a ﬁle called energy containing the energy of the structure per unit cell of the structure (not

the lattice) (this is what ﬁrst-principles code usually give anyways).

• If the calculation fails,no energy ﬁle should not be created.Instead,an empty ﬁle called error should

be created.

3.3.INTERFACING MAPS WITH OTHER FIRST-PRINCIPLES CODES 13

The above ﬁles must all reside in the current directory (from where the script was invoked).To follow

the philosophy of the package,the additional input parameters (besides the structure geometry) needed by

the ﬁrst-principles code should be contained in a ﬁle called xxx.wrap located one (or two) levels up in the

directory hierarchy,relative to the current directory.

As a starting point to write this script,have a look at the ﬁle atat/glue/vasp/runstruct

vasp.

14 CHAPTER 3.GETTING STARTED

Chapter 4

Version History and Bugs

1.50:

constituent strain

allow any structure names

allow new structures to be added at all times

1.66:

unit cell in ’symmetric’ form,ready for ab-initio codes

constituent strain fitting code

temperature-dependent ECI in Monte Carlo code

manual in tex/html

reciprocal space Monte-Carlo (BETA)

easy-to-configure job control scripts

2.03:

vibrational and electronic entropy included.

2.50:

mixed canonical/grandcanonical multicomponent monte carlo

2.53:

reciprocal space multicomponent monte carlo (for electrostatics)

2.54:

automated patching system for c++ language qwirks

2.70:

tensorial/generalized cluster expansion (gce utility)

2.71:

fixed bug in multisublattice structure enumeration routine

(only affects cases where a pure translation maps one sublattice onto another:

omits some structures with lattice vector equal to one of the unit cell lattice vectors

cluster expansions not affected,but perhaps missed ground states or SQS,but unlikely)

15

16 CHAPTER 4.VERSION HISTORY AND BUGS

Chapter 5

User guide

5.1 Introduction

First-principles calculations of alloy thermodynamic properties have been successfully employed in a variety

of contexts for metallic,semi-conductor and ceramic systems,including the computation of:composition-

temperature phase diagrams,thermodynamic properties of stable and metastable phases,short-range order

in solid solutions,thermodynamic properties of planar defects (including surfaces or antiphase and interphase

boundaries),and the morphology of precipitate microstructures [6,5,27,28,25,3,1].

Although the formalism that allows the calculation of thermodynamic properties from ﬁrst principles

has been known for decades [6,5,27],its practical implementation remains tedious.These practical issues

limit the accuracy researchers are able to obtain without spending an unreasonable amount of their time

writing input ﬁles for various computer codes,monitoring their execution and processing their output.

These practical diﬃculties also limit the community of researchers that use these methods solely to those

that possess the necessary expertise to carry out such calculations.

The Alloy Theoretic Automated Toolkit (ATAT) [22] drastically simpliﬁes the practical use of these

methods by implementing decision rules based on formal statistical analysis that free the researchers from

a constant monitoring during the calculation process and automatically “glues” together the input and

the output of various codes,in order to provide a high-level interface to the calculation of thermodynamic

properties from ﬁrst principles.In order the make this powerful toolkit available to the wide community of

researchers who could beneﬁt from it,this article present a concise user guide to this toolkit.

5.2 Theoretical Background

While there exist numerous methodologies that enable the calculation of thermodynamic properties fromﬁrst

principles,we will focus on the following two-step approach (see Figure 5.1).First,a compact representation

of the energetics of an alloy,known as the cluster expansion [18,6,5,27],is constructed using ﬁrst-principles

calculations of the formation energies of various atomic arrangements.Second,the cluster expansion is used

as a Hamiltonian for Monte Carlo simulations [16,2,8,15] that can provide the thermodynamic properties

of interest,such as the free energy of a phase or short-range-order parameters as a function of temperature

and concentration.This two-step approach is essential,because the calculation of thermodynamic quantities

through Monte Carlo involves averaging the property of interest over many diﬀerent atomic conﬁgurations

and it would be infeasible to calculate the energy of each of these conﬁgurations from ﬁrst principles.The

cluster expansion enables the prediction of the energy of any conﬁguration fromthe knowledge of the energies

of a small number of conﬁgurations (typically between 30 and 50),thus making the procedure amenable to

the use of ﬁrst-principles methods.

Formally,the cluster expansion is deﬁned by ﬁrst assigning occupation variables σ

i

to each site i of the

parent lattice,which is deﬁned as the set of all the atomic sites that can be occupied by one of a few possible

atomic species.In the common case of a binary alloy system,the occupation variables σ

i

take the value

−1 or +1 depending on the type of atom occupying the site.A particular arrangement of these “spins” on

17

18 CHAPTER 5.USER GUIDE

the parent lattice is called a conﬁguration and can be represented by a vector σ containing the value of the

occupation variable for each site in the parent lattice.Although we focus here on the case of binary alloys,

this framework can be extended to arbitrary multicomponent alloys (the appropriate formalism is presented

in [18]).

The cluster expansion then parametrizes the energy (per atom) of the alloy as a polynomial in the

occupation variables:

E(σ) =

α

m

α

J

α

i∈α

′

σ

i

(5.1)

where α is a cluster (a set of sites i).The sum is taken over all clusters α that are not equivalent by a

symmetry operation of the space group of the parent lattice,while the average is taken over all clusters

α

′

that are equivalent to α by symmetry.The coeﬃcients J

α

in this expansion embody the information

regarding the energetics of the alloy and are called the eﬀective cluster interaction (ECI).The multiplicities

m

α

indicate the number of clusters that are equivalent by symmetry to α (divided by the number of lattice

sites).

It can be shown that when all clusters α are considered in the sum,the cluster expansion is able to

represent any function E(σ) of conﬁguration σ by an appropriate selection of the values of J

α

.However,

the real advantage of the cluster expansion is that,in practice,it is found to converge rapidly.An accuracy

that is suﬃcient for phase diagram calculations can be achieved by keeping only clusters α that are relatively

compact (e.g.short-range pairs or small triplets).The unknown parameters of the cluster expansion (the

ECI) can then be determined by ﬁtting them to the energy of a relatively small number of conﬁgurations

obtained through ﬁrst-principles computations.This approach is known as the Structure Inversion Method

(SIM) or the Collony-Williams [4] method.

The cluster expansion thus presents an extremely concise and practical way to model the conﬁgurational

dependence of an alloy’s energy.A typical well-converged cluster expansion of the energy of an alloy consists

of about 10 to 20 ECI and necessitates the calculation of the energy of around 30 to 50 ordered structures (see,

for instance,[24,9,17]).Once the cluster expansion has been constructed,the energy of any conﬁguration

can be calculated using Equation 5.1 at a very small computational cost.This enables the use of various

statistical mechanical techniques such as Monte Carlo simulations [2],the low-temperature expansion (LTE)

[11,6],the high-temperature expansion (HTE) [6],or the cluster variation method (CVM) [10,6] to calculate

thermodynamic properties and phase diagrams.The atat software implements Monte Carlo simulations,

the LTE and the HTE.

Paralleling the two-step approach described in the previous section,atat consists of two main computer

programs (see Figure 5.1).The cluster expansion construction is performed by the MIT Ab initio Phase

Stability (MAPS) code [23],while the Monte Carlo simulations are driven by the Easy Monte Carlo Code

(EMC2),developed at Northwestern University [21].Each of these codes will be discussed in turn.

While the present user guide describes how the atat software can be used to carry out all the steps

necessary for the calculation of thermodynamic properties from ﬁrst principles,it must be emphasized that

each part of the toolkit can be used as a stand-alone code.For instance,many users may have access to

an existing cluster expansion obtained through the SIM or other popular methods,such as concentration-

wave-based methods (see,for instance,[7,6,20]).It is then staightforward to setup the appropriate input

ﬁles to run the emc2 Monte Carlo code.Alternatively,after obtaining a cluster expansion using the maps

code,users could choose to calculate thermodynamic properties with the cluster variation method (CVM)

[10,6],as implemented in the IMR-CVM code [19].The modularity of the toolkit actually extends below the

level of the maps and emc2 codes —many of the subroutines underlying these codes can be accessed through

stand-alone utilities [22].

5.3 Cluster expansion construction using the MAPS code

The maps code implements the so-called Structure Inversion Method (SIM),also known as the Connolly-

Williams method [4].While the algorithms underlying the maps code are described in [23],the present

section focuses on its practical use.

5.3.CLUSTER EXPANSION CONSTRUCTION USING THE MAPS CODE 19

Figure 5.1:Methodology implemented in atat for the computation of thermodynamic properties from ﬁrst

principles.The automated construction of the cluster expansion is performed by the maps code.Whenever

needed,maps requests the calculation of the formation energy of various atomic conﬁgurations by a ﬁrst-

principles code (such as vasp).The necessary input ﬁles are created and the resulting output ﬁles are parsed

without requiring user intervention.The output of maps is a set of eﬀective cluster interactions that deﬁne a

computationally eﬃcient Hamiltonian that can be used to perform Monte Carlo simulations with the emc2

code.These simulations provide thermodynamic properties and phase diagrams that can be used to create

thermodynamic databases or supplement existing ones.

Cluster expansion construction

MAPS

(MIT Ab-initio

Phase Stability Code)

Monte Carlo Simulations

Emc2

(Easy Monte Carlo Code)

Lattice geometry

Ab-initio code parameters

Thermodynamic quantities

Phase diagrams

Effective cluster interactions

(ECI)

Ab-initio code

ex: VASP

5.3.1 Input ﬁles

The maps code needs two input ﬁles:one that speciﬁes the geometry of the parent lattice (lat.in) and

one that provides the parameters of the ﬁrst-principles calculations (xxxx.wrap,where xxxx is the name

of the ﬁrst-principles code used).The clear separation between the thermodynamic and ﬁrst-principles

calculations is a distinguishing feature of atat that enables the package to be easily interfaced with any

ﬁrst-principles code.Table 5.1 gives two annotated examples of a lattice geometry input ﬁle.The package

includes ready-made lattice ﬁles for the common lattice types (e.g.bcc,fcc,hcp).It also includes an utility

that automatically constructs multiple lattice geometry input ﬁles for common lattices.For instance,

makelat Al,Ti fcc,bcc,hcp

creates 3 subdirectories containing the appropriate input ﬁles for each speciﬁed lattice.

The ﬁrst-principles input ﬁle is usually less than 10 lines long,thanks to the dramatic improvements in

the user-friendliness of most modern ﬁrst-principles codes.For instance,in the case of the widely used VASP

code [13,12],a typical input ﬁle is given in Table 5.2.Examples of such input ﬁles are provided with the

package.Note that atat contains a utility that enables the automatic construction of k-point meshes from

a single parameter deﬁning the desired target k-point density,the number of k-point per reciprocal atom

(KPPRA).

5.3.2 Running the code

The maps code is started using the command

20 CHAPTER 5.USER GUIDE

Table 5.1:Examples of lattice geometry input ﬁle lat.in.Typically,the coordinate system entry is used to

deﬁne the conventional unit cell so that all other entries can be speciﬁed in the normalized coordinates that

are the most natural for the symmetry of the lattice.The input lattice parameters do not need to be exact,

as the ﬁrst-principles code will optimize them.

Example 1:hcp Ti-Al system

3.1 3.1 5.062 90 90 120 (Coordinate system:a b c α β γ notation)

1 0 0 (Primitive unit cell:one vector per line

0 1 0 expressed in multiples of the above coordinate

0 0 1 system vectors)

0 0 0 Al,Ti (Atoms in the lattice)

0.6666666 0.3333333 0.5 Al,Ti

Example 2:rocksalt CaO-MgO pseudobinary system

4.1 4.1 4.1 90 90 90

0 0.5 0.5

0.5 0 0.5

0.5 0.5 0

0 0 0 Ca,Mg (“Active” atoms in the lattice)

0.5 0.5 0.5 O (“spectator” ion)

Table 5.2:Examples of ﬁrst-principles code input ﬁle (example given for the vasp code).It is especially

important to verify that the KPPRA parameter is set suﬃciently large for the system under study.

[INCAR]

PREC = high

ENMAX = 200

ISMEAR = -1

SIGMA = 0.1

NSW=41

IBRION = 2

ISIF = 3 (See vasp manual for a description of the above 6 parameters.)

KPPRA = 1000 (Sets the k-point density (K Point Per Reciprocal Atom))

DOSTATIC (Performs a “static run” — see vasp manual)

maps -d &

where the option -d indicates that all default values of the input parameters should be used,which is

what most users will ever need.(The optional parameters can be displayed by typing maps by itself and

further help is available via the command maps -h.) The trailing & character cause the command to execute

in “background” mode.In this fashion,maps can continuously be on the lookout,responding to various

“signals”,while the user performs other tasks.(The ongoing discussion assumes that the code is run under

a UNIX environment within a shell such as sh,csh,tcsh or bash.)

The process of constructing a cluster expansion from ﬁrst-principles calculations can be summarized as

follows.

1.Determine the parameters of the ﬁrst-principles code that provide the desired accuracy.

2.Let maps reﬁne the cluster expansion.

3.Decide when the cluster expansion is suﬃciently accurate.

5.3.CLUSTER EXPANSION CONSTRUCTION USING THE MAPS CODE 21

Typically,one calibrates the accuracy of the ﬁrst-principles calculations using the “pure”

1

structures of

the alloy system of interest.To generate the two “pure” structures,type

touch ready

This creates a ﬁle called ready which tells maps that you are ready to calculate the energy of a structure.

Within 10 seconds,maps replies with

Finding best structure...

done!

maps has just created a directory called 0 and,within it,a ﬁle called str.out that contains the geometry of

one of the two “pure” structures.If you type touch ready once more,the other “pure” structure is written

to 1/str.out.You now need to launch the ﬁrst-principles code to calculate the energy of each structure.

Type

cd 0

to go into the directory of the ﬁrst structure.Assuming that your ﬁrst-principles code is called xxxx,type

runstruct

xxxx &

After this command has successfully terminated,display the energy of that structure and go back to the

initial directory

cat energy

cd..

and edit the ﬁle deﬁning the ﬁrst-principles code parameters

emacs xxxx.wrap &

so that the precision of the calculation is increased (e.g.increase the k-point density or the cut-oﬀ of the

plane-wave energy).Then you rerun the calculations to check by how much the calculated energy has

changed:

cd 0

runstruct

xxxx &

cat energy (After the calculations are completed)

cd..

This process is repeated until the user is satisﬁed with the precision of the calculation (that is,if the energy

has become insensitive to changes in the input parameters within the desired accuracy).

2

A similar study

should also be performed for the other “pure” structure (labeled structure 1) and,if one is really concerned

with precision,for a few structures with intermediate concentrations.

Once the appropriate ab initio code parameters have been determined,the fully automated process can

begin.From within the directory where maps was started,type

pollmach runstruct

xxxx

to start the job manager that will monitor the load on your local network of workstations and ask maps

to generate new structures (i.e.atomic arrangements) whenever a processor becomes available.Note that

the ﬁrst time the command is run,instructions will appear on screen that explain how to conﬁgure the job

dispatching system in accordance to your local computing environment.Once this conﬁguration is complete,

the above command should be invoked in the background by appending a “&” to it.

1

In the case of pseudobinary alloys with spectator ions (e.g.the MgO-CaO system),the “pure” structures would correspond

to the structures where the sublattice of interest is entirely ﬁlled with a single type of atom.

2

A key number to keep in mind is that an error of 25meV corresponds to 300K on a temperature scale.

22 CHAPTER 5.USER GUIDE

5.3.3 Output of MAPS

While the calculations are running,you can check on the status of the best cluster expansion obtained so far.

The ﬁle log.out contains a brief description of the status of the calculations,such as the accuracy of the

cluster expansion and various warning messages.Most of the messages pertains to the accurate prediction

of the so-called ground states of the alloy system.The ground states,which are the structures that have

the lowest energy for each given concentration,are extremely important to predict accurately because they

determine which phases will appear on the phase diagram.The four possible messages are described below.

• Not enough known energies to fit CE.Before displaying any results,maps waits until enough

structural energies are known to ﬁt a minimal cluster expansion containing only nearest-neighbor

pair interactions and test its accuracy.Thus,the ﬁrst cluster expansion is typically constructed after

at least 4 structural energies have been computed (this number may vary as a function of the symmetry

of the lattice).

• Among structures of known energy,true ground states differ from fitted ground

states.The current cluster expansion incorrectly predicts which structures have the lowest energy for

given concentrations,among structures whose ﬁrst-principles energy is known.The code has built-in

checks to avoid this.However,in rare instances,it may be mathematically impossible to satisfy all

the constraints that the code imposes for a cluster expansion to be acceptable.This problem becomes

increasingly unlikely as the number of calculated structural energies increases,so the user should just

wait until the problem ﬁxes itself.

• Among structures of known energy,true and predicted ground states agree.Opposite of

the previous message.When this message is displayed,maps also displays either one of the following

two messages.

• New ground states of volume less or equal to n predicted,see predstr.out.This indi-

cates that the cluster expansion predicts that,at some concentration,there exist other structures

that should have an energy even lower than the one of the structures whose energy has been calculated

from ﬁrst principles.In this case,maps will investigate the matter by generating those structures and

requesting that their energy be calculated.Once again,the user should just wait for the problem to ﬁx

itself.The predicted ground states are ﬂagged by a g in the predstr.out ﬁle,so that you can display

their energy by typing

grep g predstr.out

• No other ground states of n atoms/unit cell or less exist.The energies of all ground states

predicted by the cluster expansion have been conﬁrmed by ﬁrst-principles calculations.Because it can

be computationally intensive to perform a full ground state search when interactions extend beyond

the nearest-neighbor shell [6],maps uses a search algorithm that merely enumerates every possible

structures having n atoms or less per unit cell and uses the cluster expansion to predict their energies.

The upper limit n increases automatically as calculations progress.

The log.out ﬁle also contains two other pieces of information:

• Concentration range used for ground state checking:[a,b] This displays the user-selected

range of concentration over which ground state checking is performed (which can be speciﬁed as a

command-line option of the maps command:-c0=a -c1=b).It may be useful to relax the constraints

that ground states be correctly reproduced over the whole concentration range when it is known that

other parent lattices are stable in some concentration range.In this fashion,the code can focus on

providing a higher accuracy in the concentration range where the user needs it.

• Crossvalidation score:s.This provides the predictive power of the cluster expansion.It is analo-

gous to the root mean square error,except that it is speciﬁcally designed to estimate the error made

in predicting the energy for structures not included in the least-squares ﬁt [23].It is deﬁned as

CV =

1

n

n

i=1

E

i

−

ˆ

E

(i)

2

1/2

5.4.MONTE CARLO SIMULATIONS 23

where E

i

is the calculated energy of structure i,while

ˆ

E

(i)

is the predicted value of the energy of

structure i obtained from a least-squares ﬁt to the (n −1) other structural energies.

The maps code also outputs quantitative data in various output ﬁles.The simplest way to analyze this data

is by typing

mapsrep

As illustrated in Figure 5.2,this command displays,in turn

• The log.out ﬁle described earlier.

• The formation energy of all structures whose energy is known from ﬁrst-principles calculations,as well

as the predicted energy of all structures maps has in memory.The convex hull of the ground states

among structures of known energy is overlaid while the new predicted ground states (if any) are marked

by an “×”.(Note that this ground state line is only meaningful if the log.out ﬁle contains “Among

structures of known energy,true and predicted ground states agree.”)

• The formation energy of all structures calculated from ﬁrst principles and associated ground state line.

• A plot of the magnitude of the Eﬀective Cluster Interactions (ECI) as a function of the diameter

of their associated cluster (deﬁned as the maximum distance between any two sites in the cluster).

Pairs,triplets,etc.are plotted consecutively.This plot is useful to assess the convergence of the

cluster expansion.When the magnitude of the ECI for the larger clusters has clearly decayed to a

negligible value (relative to the nearest-neighbor pair ECI),this is indicative of a well-converged cluster

expansion.

• A plot of the residuals of the ﬁt (i.e.the ﬁtting error) for each structure.This information is useful to

locate potential problems in the ﬁrst-principles calculations.Indeed,when ﬁrst-principles calculations

exhibit numerical problems,this typically results in calculated energies that are poorly reproduced by

the cluster expansion.

When the user is satisﬁed with the results (which are constantly updated),maps can be stopped by

creating a ﬁle called stop in the current directory using the command:

touch stop

while the job dispatching system can be stopped by typing:

touch stoppoll

A cluster expansion can be considered satisfactory when

1.All ground states are correctly reproduced and no new ground states are predicted.(The log.out

ﬁle would then indicate that Among structures of known energy,true and predicted ground

states agree.No other ground states of n atoms/unit cell or less exist.)

2.The crossvalidation score,as given in the log.out ﬁle,is small (typically less than 0.025 eV).

3.Optionally,it is instructive to verify that the magnitude of the ECI decays as a function of the diameter

of the corresponding cluster and as a function of the number of sites it contains.

5.4 Monte Carlo simulations

The emc2 code implements semi-grand canonical Monte Carlo simulations [16,2,8,15],where the total

number of atoms is kept ﬁxed,while the concentration is allowed to adapt to an externally imposed diﬀerence

in the chemical potential of the two types of atoms.The chemical potential diﬀerence will be simply referred

to as the “chemical potential” in what follows.This ensemble oﬀers the advantage that,for any imposed

24 CHAPTER 5.USER GUIDE

Figure 5.2:Output of the maps Code,as reported by the mapsrep command.a) Energies predicted from the

cluster expansion as a function of composition for each structure generated.“known str” denotes structures

whose energy has been calculated from ﬁrst principles.“known gs” indicate the ground states that have

so far been conﬁrmed by ﬁrst-principles calculations and the dashed line outlines the convex hull of the

ground states,which serves as a threshold to detect other candidate ground states.“predicted” denotes

structures whose energy has not yet been calculated from ﬁrst principles.“predicted gs” are structures

that are predicted by the cluster expansion to be ground states,although this prediction has not yet been

conﬁrmed by ﬁrst-principles calculations.b) Energies calculated from ﬁrst principles.“known str” and

“known gs” are as in a),except that the energy calculated from ﬁrst principles is reported.c) Eﬀective

Cluster Interaction (ECI) as a function of the diameter of the associated cluster and as a function of the

number of sites in the cluster (i.e.pair,triplet,etc.).d) Residuals of the ﬁt,that is,the diﬀerence between

the ﬁrst-principles energies and the energies predicted from the cluster expansion.(The abscissa refers to

the line number within the output ﬁle fit.out listing all the structures with known energies.)

-0.45

-0.4

-0.35

-0.3

-0.25

-0.2

-0.15

-0.1

-0.05

0

0

0.2

0.4

0.6

0.8

1

Calculated Energies

known str

known gs

-0.02

-0.01

0

0.01

0.02

0.03

0.04

0.05

0.06

pair

5

10

15

trip

5

10

15

quad

5

10

15

ECI vs cluster diameter

-0.04

-0.02

0

0.02

0.04

0.06

0.08

0

10

20

30

40

50

60

Residuals of the fit (same order as in fit.out)

a) b)

d)

c)

-0.45

-0.4

-0.35

-0.3

-0.25

-0.2

-0.15

-0.1

-0.05

0

0

0.2

0.4

0.6

0.8

1

Fitted Energies

predicted

known str

known gs

predicted gs

chemical potential,the equilibrium state of the system is a single phase equilibrium,free of interfaces.

3

It

also simpliﬁes the process of calculating free energies through thermodynamic integration.While a detailed

description of the algorithm underlying this code can be found in [21],the current section focuses on the

practical usage of the code.

3

If the simulation cell is commensurate with the unit cell of the phase under study,a requirement that the code automatically

ensures.

5.4.MONTE CARLO SIMULATIONS 25

5.4.1 General input parameters

The Monte Carlo code needs the following ﬁles as an input

1.A lattice geometry ﬁle (lat.in),which is the same as the input for maps (see Table 5.1).

2.Files providing the cluster expansion (the clusters used are listed in the clusters.out ﬁle while the

corresponding ECI are listed in the eci.out ﬁle.).These ﬁles are automatically generated by maps,

although users can supply their own cluster expansion,if desired.A description of the format of these

ﬁles is available by typing maps -h.

3.A list of ground states (gs

str.out),which merely provide convenient starting conﬁgurations for the

simulations.maps also automatically creates this ﬁle.

The parameters controlling the simulation are speciﬁed as command-line options.The ﬁrst input param-

eter(s) needed by the code are the phase(s) whose thermodynamic properties are to be determined.There

are two ways to invoke the Monte Carlo simulation code.When the command emc2 is used,a single Monte

Carlo simulation is run to allow the calculation of thermodynamic properties of a single phase for the whole

region of chemical potential and temperature where that phase is stable.The phase of interest is speciﬁed

by a command-line option of the form

-gs=n,

where n is a number between −1 and G−1 (inclusive),where G is the number of ground states.The value

−1 indicates the disordered phase while values ranging from 0 to G−1 indicate the phases associated with

each ground states (0 denoting the ground state with the smallest composition).When the command phb is

used,two Monte Carlo simulations are run simultaneously to enable the determination of the temperature-

composition phase boundary associated with a given two-phase equilibrium.The two phases are speciﬁed

by

-gs1=n

1

-gs2=n

2

.

It is possible to compute a two-phase equilibrium between phases deﬁned on a diﬀerent parent lattice.In

this case,the user needs to specify the directories where the cluster expansions of each lattice resides using

the options of the form

-d1=directory 1 -d2=directory 2

The accuracy of the thermodynamic properties obtained from Monte-Carlo simulations is determined by

two parameters:The size of the simulation cell and the duration of the simulation.

The size of the simulation cell is speciﬁed by providing the radius r of a sphere through the command-line

option

-er=r.

As illustrated in Figure 5.3a,the simulation cell size will be the smallest supercell that both contains

that sphere and that is commensurate with the unit cell of the ground state of interest.This way of

specifying the simulation cell size ensures that the systemsize is comparable along every direction,regardless

of the crystal structure of the ground state of interest.It also frees the user from manually checking the

complicated requirement of commensurability.It is important that the user check that the simulation cell

size is suﬃciently large for the thermodynamic properties of interest to be close to their inﬁnite-system-size

limiting value.This can be done by gradually increasing the system size until the calculated quantities

become insensitive to the further increases in system size,within the desired accuracy.

The duration of the simulations is automatically determined by the code from a user-speciﬁed target

precision on the atomic composition of the phase,indicated by a command-line option of the form

-dx=Δx.

Alternatively,the user may also manually set the number n

eq

of Monte Carlo steps the system is allowed to

equilibrate before thermodynamic averages are computed over a certain number n

avg

of Monte Carlo steps

using the options

26 CHAPTER 5.USER GUIDE

Figure 5.3:Deﬁnitions of the quantities used to specify a) the simulation cell size and b) the chemical

potential.

a)

b)

Unit cell

Simulation Cell

r

0

0.2

0.4

0.6

0.8

1

Concentration

0

1

2

3

4

5

=1

=2

=3

=4

=5

= 3.5

Energy

-eq=n

eq

-n=n

avg

.

The Monte Carlo code also needs additional parameters that specify which portion of a phase’s free

energy surface needs to be computed.With emc2,the range of temperatures to be scanned are speciﬁed in

either one of the following two ways:

-T0=T

0

-T1=T

1

-dT=ΔT (for steps in direct temperature)

or -T0=T

0

-T1=T

1

-db=Δ(1/T) (for steps in reciprocal temperature).

The temperature steps in reciprocal temperature (Δ(1/T)) can be useful when calculations are started from

inﬁnite temperatures down to a ﬁnite temperature.The -T1 and -dT (or -db) options can be omitted

if calculations at a single temperature are desired.Since the program automatically stops when a phase

transition is detected,it is not necessary to know in advance the temperature range of stability of the phase.

The user only needs to ensure that the initial temperature lies within the region of stability of the phase of

interest.An obvious starting point is T

0

= 0,since the ground state is then stable,by deﬁnition.With the

phb code,the syntax is

-T=T -dT=ΔT

If the -T option is omitted,calculations start at absolute zero.

4

The energy and temperature units used are

set by specifying the Boltzman’s constant with the command-line option

-k=k

B

.

A value of 8.617 ×10

−5

corresponds to energies in eV and temperatures in Kelvin.

With emc2,the range of chemical potentials to be scanned needs to be speciﬁed.Once again,only the

starting point really matters,because the code will stop when a phase transition is reached.By default,

chemical potentials are given in a dimensionless form,so as to facilitate the link between the value of the

chemical potential and the phase that it stabilizes.For instance,a chemical potential equal to 3.0 is such

that it would stabilize a two phase equilibrium between phase number 2 and phase number 3 at absolute

zero (see Figure 5.3b).A chemical potential between 3.0 and 4.0 stabilizes phase number 3 at absolute

zero.While these ranges of stability are no longer exact at ﬁnite temperature,this dimensionless chemical

potential still provides easy-to-interpret input parameters.The syntax is

4

Temperature steps in reciprocal temperature are not needed,because a two-phase equilibrium never extents up to inﬁnite

temperature.

5.4.MONTE CARLO SIMULATIONS 27

-mu0=µ

0

-mu1=µ

1

-dmu=Δµ

where Δµ is the chemical potential step between each new simulation.Chemical potentials can also be

entered in absolute value (say in eV,if the energies are in eV) by specifying the -abs option.Note that the

output ﬁles always give the absolute chemical potentials,so that thermodynamic quantities can be computed

from them.With phb,the initial chemical potential is optional when starting from absolute zero because

the code can determine the required value from the ground state energies.It can nevertheless be speciﬁed

(in absolute value) with the -mu=µ option,if a ﬁnite temperature starting point is desired.

A list of the command line options of either the emc2 or phb codes can be displayed by simply typing

either command by itself.More detailed help is displayed using the -h option.

5.4.2 Examples

We now give simple examples of the usage of these commands.Consider the calculation of the free energy

of the phase associated with ground state number 1 as a function of concentration and temperature.Then,

the required commands could,for instance,be

emc2 -gs=1 -mu0=1.5 -mu1=0.5 -dmu=0.04 -T0=300 -T1=5000 -dT=50 -k=8.617e-5 -dx=1e-3 -er=50

-innerT -o=mc10.out

emc2 -gs=1 -mu0=1.5 -mu1=2.5 -dmu=0.04 -T0=300 -T1=5000 -dT=50 -k=8.617e-5 -dx=1e-3 -er=50

-innerT -o=mc12.out

(The only diﬀerence in the two command lines is the value of -mu1 and the output ﬁle name,speciﬁed by the

-o option.) These commands separately compute the two “halfs” of the free energy surface,corresponding to

the values of the chemical potential below and above the “middle” value of 1.5 which stabilizes ground state

1 at absolute zero.This natural separation allows you to run each half calculation on a separate processor

and obtain the results in half the time.The values of -dmu,-dT,-dx and -er given here are typical values.

The user should ensure that these values are such that the results are converged.Note that,thanks to the

way these precisions parameters are input,if satisfying values have been found for one simulation,the same

values will provide a comparable accuracy for other simulations of the same system.The option -innerT

indicates that the inner loop of the sequence of simulations scans the temperature axis while the outer loop

scans the chemical potential.In this fashion,the point of highest temperature in the region of stability of

the phase will be known early during the calculations.If the user is more interested in obtaining solubility

limits early on,this option can be omitted and the inner loop with scan the chemical potential axis.In

either cases,the code exits the inner loop (and the outer loop,if appropriate) when it encounters a phase

transition.

The emc2 code thus enables the automated calculation of the whole free energy surface of a given phase,

as illustrated in Figure 5.4a.Such free energy surfaces can be used as an input to construct thermodynamic

databases or supplement existing ones.To facilitate this process,a utility that converts the output of emc2

into input ﬁles for the ﬁtting module of ThermoCalc is provided.

While the above examples focus on the calculation of a phase’s thermodynamic properties over its whole

region of stability,one may be interested in directly computing the temperature-composition phase boundary

without ﬁrst constructing a full free energy surface.To accomplish this task,a typical command-line for the

phb program would be

phb -gs1=0 -gs2=1 -dT=25 -dx=1e-3 -er=50 -k=8.617e-5 -ltep=5e-3 -o=ph01.out

This command computes the two phase equilibrium between phase 0 and phase 1,starting at absolute

zero and incrementing temperature in steps of 25 K.(The -ltep option indicates that a Low Temperature

Expansion (LTE) should be used instead of Monte Carlo simulation whenever its precision is better than

5 ×10

−3

eV.) The output ﬁle ph01.out contains the temperature-composition phase boundary of interest,

as well as the chemical potential stabilizing the two-phase equilibrium as a function of temperature.This

output can be used to generate phase diagrams,as illustrated in Figure 5.4b.

The program automatically terminates when the “end” of the two-phase equilibrium has been reached.

If the two-phase equilibrium disappears because of the appearance of a third phase,two new two-phase

equilibria have to be separately calculated.To do so,one uses the ﬁnal temperature T and chemical potential

µ given in the output ﬁle as a starting point for two new phb runs:

28 CHAPTER 5.USER GUIDE

Figure 5.4:Output of Monte Carlo codes.a) The emc2 provides free energy surfaces as a function of

temperature T and composition x.(For clarity,the common tangent construction (thick lines) is drawn over

the calculated free energy.) b) The phb command generates temperature-composition phase diagrams.The

calculational details underlying these results can be found in [23,21]

a)

b)

phb -T=T -mu=µ -gs1=0 -gs2=-1 -dT=25 -dx=1e-3 -er=50 -k=8.617e-5 -o=ph0d.out

phb -T=T -mu=µ -gs1=-1 -gs2=1 -dT=25 -dx=1e-3 -er=50 -k=8.617e-5 -o=phd1.out

In the above example,it is assumed that the new phase appearing is the disordered phase (indicated by the

number −1),which will usually be the case.Of course,it is also possible that a given two-phase equilibrium

terminates because one of the two phases disappears.In this case,only one new calculation needs to be

started,as in the following example:

phb -T=T-mu=µ -gs1=0 -gs2=2 -dT=25 -dx=1e-3 -er=50 -k=8.617e-5 -o=phd1.out

Note that phase 1 has been replaced by phase 2.Finally,it is also possible that the two-phase equilibrium

terminates because the concentration of each phase converges to the same value,a situation which requires

no further calculations.The user can easily distinguish these three cases by merely comparing the ﬁnal

composition of each phase.

5.4.3 Interpreting the output ﬁles

The output ﬁle of emc2 reports the value of all calculated thermodynamic functions for each value of tem-

perature and chemical potential scanned.The quantities reported include

• Statistical averages over Monte Carlo steps,such as energy,concentration,short-range and long-range

order parameters.

5

• Integrated statistical averages,such as the Gibbs free energy G or the semi-grand-canonical potential

φ = G−µx.

• The result of common approximations,namely,the low temperature expansion (LTE) [6,11,26],the

mean-ﬁeld (MF) approximation and the high temperature expansion (HTE) (see,for instance,[6]).

While quantities obtained from statistical averages over Monte Carlo steps are valid for all temperatures and

chemical potentials,caution must be exercised when interpreting the result of the various approximations

or when looking at the integrated quantities.The LTE,MF and HTE approximations are only accurate

in a limited range of temperature and it is the responsibility of the user to assess this range of validity.

5

For eﬃciency reasons,the long range order parameters are only calculated when starting from an ordered phase.

5.5.RECENT DEVELOPMENTS 29

Also,the free energy or the semi-grand-canonical potential are obtained from thermodynamic integration

and are thus only valid if the starting point of the integration is chosen appropriately.By default,the low

temperature expansion value is used as a starting point whenever the phase of interest is a ground state,

while the high temperature expansion is used when the phase of interest is the disordered state.Hence,

to obtain absolute values of the semi-grand-canonical potential,one must ensure that the calculations are

started at a suﬃciently low temperature (or suﬃciently high temperature,in the case of the disordered

phase).This can be checked by comparing the Monte Carlo estimates with the LTE (or HTE) estimates and

verifying that they agree for the ﬁrst few steps of the thermodynamic integration.A user-speciﬁed starting

point for φ (e.g.obtained from an earlier Monte Carlo simulation) can be indicated using the option

-phi0=φ

Note that,unlike emc2,the phb code automatically makes use of the low temperature expansion whenever

it is suﬃciently accurate in order to save a considerable amount of computational time.

By default,the code reports the thermodynamic quantities associated with the semi-grand-canonical

ensemble,such as the semi-grand-canonical potential φ.The command-line option -can,instructs the code

to add µx to all appropriate thermodynamic quantities,so that the code outputs the more commonly used

canonical quantities,such as the Gibbs free energy G and the internal energy E.

5.5 Recent developments

The multicomponent version of maps is mmaps and the multicomponent version of emc2 is memc2.The phb

code does not have a multicomponent version.All other utilities can handle multicomponent systems.

Although the present tutorial does not discuss the topic,atat also implements reciprocal space cluster

expansions and,in particular,the constituent strain formalism [14],see the command reference for csfit.

atat can also calculate nonconﬁgurational contributions to the free energy,such as lattice vibrations and

electronic excitations,see the command reference for fitsvsl,svsl,fitfc and felec.

5.6 Conclusion

The Alloy Theoretic Automated Toolkit (ATAT) drastically simpliﬁes the practical implementation of the

Connolly-Williams method,in combination with semi-grand-canonical Monte Carlo simulations,thus pro-

viding a high-level interface to the calculation of thermodynamic properties fromﬁrst principles.This toolkit

enables researcher to focus on higher-level aspects of ﬁrst-principles thermodynamic calculations by encap-

sulating the intricate details of the calculations under an easy-to-use interface.It also makes these powerful

methodologies readily available to the wide community of researchers who could beneﬁt from it.

30 CHAPTER 5.USER GUIDE

Bibliography

[1] M.Asta,V.Ozolins,and C.Woodward.A ﬁrst-principles approach to modeling alloy phase equilibria.

JOM - Journal of the Minerals Metals & Materials Society,53:16,2001.

[2] K.Binder and D.W.Heermann.Monte Carlo Simulation in Statistical Physics.Springer-Verlag,New

York,1988.

[3] G.Ceder,A.van der Ven,C.Marianetti,and D.Morgan.First-principles alloy theory in oxides.

Modelling Simul.Mater Sci Eng.,8:311,2000.

[4] J.W.Connolly and A.R.Williams.Density-functional theory applied to phase transformations in

transition-metal alloys.Phys.Rev.B,27(8):5169,1983.

[5] D.de Fontaine.Cluster approach to order-disorder transformation in alloys.Solid State Phys.,47:33,

1994.

[6] F.Ducastelle.Order and Phase Stability in Alloys.Elsevier Science,New York,1991.

[7] F.Ducastelle and F.Gautier.Generalized perturbation-theory in disordered transitional alloys —

application to calculation of ordering energies.Journal of Physics F — Metal Physics,6:2039,1976.

[8] B.D¨unweg and D.P.Landau.Phase diagram and critical behavior of the si-ge unmixing transition:A

monte carlo study of a model with elastic degrees of freedom.Phys.Rev.B,48:14182,1993.

[9] G.D.Garbulksy and G.Ceder.Linear-programming method for obtaining eﬀective cluster interactions

in alloys from total-energy calculations:application to the fcc pd-v system.Phys.Rev.B,51(1):67,

1995.

[10] R.Kikuchi.A theory of cooperative phenomena.Phys.Rev.,81:988,1951.

[11] A.F.Kohan,P.D.Tepesch,G.Ceder,and C.Wolverton.Computation of alloy phase diagrams at low

temperatures.Comput.Mater.Sci.,9:389,1998.

[12] G.Kresse and J.Furthm¨uller.Eﬃciency of ab-initio total energy calculations for metals and semicon-

ductors using a plane-wave basis set.Comput.Mater.Sci.,6:15,1996.

[13] G.Kresse and J.Furthm¨uller.Eﬃcient iterative schemes for ab initio total-energy calculations using a

plane-wave basis set.Phys.Rev.B,54:11169,1996.

[14] D.B.Laks,L.G.Ferreira,S.Froyen,and A.Zunger.Eﬃcient cluster expansion for substitutional

systems.Physical Review B,46:12587,1992.

[15] M.Laradji,D.P.Landau,and B.D¨unweg.Structural properties of Si

1−x

Ge

x

alloys:A monte carlo

simulation with the stillinger-weber potential.Phys.Rev.B,51:4894,1995.

[16] M.E.J.Newman and G.T.Barkema.Monte Carlo Methods in Statistical Physics.Clarendon Press,

Oxford,1999.

[17] V.Ozoli¸nˇs,C.Wolverton,and A.Zunger.Cu-au,ag-au,cu-ag,and ni-au intermetallics:First-principles

study of temperature-composition phase diagrams and structures.Phys.Rev.B,57:6427,1998.

31

32 BIBLIOGRAPHY

[18] J.M.Sanchez,F.Ducastelle,and D.Gratias.Generalized cluster description of multicomponent sys-

tems.Physica,128A:334,1984.

[19] M.H.Sluiter.Imr-cvm code,2000.http://www-lab.imr.tohoku.ac.jp/˜marcel/cvm/cvm.html.

[20] P.E.A Turchi.In J.H.Westbrook and R.L.Fleisher,editors,Intermetallic Compounds:Principles

and Practice,volume 1,page 21,New York,1995.John Wiley.

[21] A.van de Walle and M.Asta.Self-driven lattice-model monte carlo simulations of alloy thermodynamic

properties and phase diagrams.Modelling Simul.Mater.Sci.Eng.,10:521,2002.

[22] A.van de Walle,M.Asta,and G.Ceder.Invited paper:The alloy theoretic automated toolkit:A

user guide.CALPHAD Journal,26:539,2002.

[23] A.van de Walle and G.Ceder.Automating ﬁrst-principles phase diagram calculations.Journal of

Phase Equilibria,23:348,2002.

[24] A.van der Ven,M.K.Aydinol,G.Ceder,G.Kresse,and J.Hafner.First-principles investigation of

phase stability in li

x

coo

2

.Phys.Rev.B,58:2975,1998.

[25] C.Wolverton,V.Ozoli¸nˇs,and A.Zunger.Short-range-order types in binary alloys:a reﬂection of

coherent phase stability.J.Phys.:Condens.Matter,12:2749,2000.

[26] C.Woodward,M.Asta,G.Kresse,and J.Hafner.Density of constitutional and thermal point defects

in L1

2

Al

3

Sc.Phys.Rev.B,63:094103,2001.

[27] A.Zunger.First principles statistical mechanics of semiconductor alloys and intermetallic compounds.In

P.E.Turchi and A.Gonis,editors,NATO ASI on Statics and Dynamics of Alloy Phase Transformation,

volume 319,page 361,New York,1994.Plenum Press.

[28] A.Zunger.Spontaneous atomic ordering in semiconductor alloys:Causes,carriers,and consequences.

MRS Bull.,22:20,1997.

Chapter 6

Interfacing with ThermoCalc

A description of the steps necessary to convert the output of the Monte Carlo code emc2 to input ﬁles

suitable for the PARROT module of ThermoCalc are described in an online tutorial by Gautam Ghosh

available at:http://www.its.caltech.edu/˜avdw/atat/emc2tc.pdf.These steps are partially automated in

the script atat/glue/tc/emc2tc included in the ATAT distribution.

33

34 CHAPTER 6.INTERFACING WITH THERMOCALC

Chapter 7

Command Reference

7.1 Man pages

7.1.1 corrdump

->What does this program do?

1) It reads the lattice file (specified by the -l option).

2) It determines the space group of this lattice and

writes it to the sym.out file.

3) It finds all symmetrically distinct clusters that satisfy the

conditions specified by the options -2 through -6.

For instance,if -2=2.1 -3=1.1 is specified,

only pairs shorter than 2.1 units and triplets containing

no pairs longer than 1.1 will be selected.

4) It writes all clusters found to clusters.out.

If the -c option is specified,clusters are read from clusters.out instead.

5) It reads the structure file (specified by the -s option).

6) It determines,for that structure,the correlations associated with all

the clusters chosen earlier.

This information is then output on one line,in the same order as in the

clusters.out file.See below for conventions used to calculate correlations.

7) It writes the files corrdump.log containting the list of all adjustements

needed to map the (possibly relaxed) structure onto the ideal lattice.

->File formats

Lattice and structure files

Both the lattice and the structure files have a similar structure.

First,the coordinate system a,b,c is specified,either as

[a] [b] [c] [alpha] [beta] [gamma]

or as:

[ax] [ay] [az]

35

36 CHAPTER 7.COMMAND REFERENCE

[bx] [by] [bz]

[cx] [cy] [cz]

Then the lattice vectors u,v,w are listed,expressed in the coordinate system

just defined:

[ua] [ub] [uc]

[va] [vb] [vc]

[wa] [wb] [wc]

Finally,atom positions and types are given,expressed in the same coordinate system

as the lattice vectors:

[atom1a] [atom1b] [atom1c] [atom1type]

[atom2a] [atom2b] [atom2c] [atom1type]

etc.

In the lattice file:

-The atom type is a comma-separated list of the atomic

symbols of the atoms that can sit the lattice site.

-In a binary,the first symbol listed is assigned a spin of -1.

In general,ordering of the atom symbol corresponds to value of s=0,1,...in the table

’Convention used to calculate the correlations’ below.

-When only one symbol is listed,this site is ignored for the purpose

of calculating correlations,but not for determining symmetry.

-The atomic symbol ’Vac’ is used to indicate a vacancy.

In the structure file:

-The atom type is just a single atomic symbol

(which,of course,has to be among the atomic symbols given in the

lattice file).

-Vacancies do not need to be specified.

Examples

The fcc lattice of the Cu-Au system:

1 1 1 90 90 90

0 0.5 0.5

0.5 0 0.5

0.5 0.5 0

0 0 0 Cu,Au

The Cu3Au L1_2 structure:

1 1 1 90 90 90

1 0 0

0 1 0

0 0 1

0 0 0 Au

0.5 0.5 0 Cu

0.5 0 0.5 Cu

0 0.5 0.5 Cu

A lattice for the Li_x Co_y Al_(1-y) O_2 system:

0.707 0.707 6.928 90 90 120

0.3333 0.6667 0.3333

-0.6667 -0.3333 0.3333

0.3333 -0.3333 0.3333

0 0 0 Li,Vac

7.1.MAN PAGES 37

0.3333 0.6667 0.0833 O

0.6667 0.3333 0.1667 Co,Al

0 0 0.25 O

Symmetry file format (sym.out)

[number of symmetry operations]

3x3 matrix:point operation

1x3 matrix:translation

repeat,etc.

Note that if you enter more than one unit cell of the lattice,

sym.out will contain some pure translations as symmetry elements.

Cluster file format (clusters.out)

for each cluster:

[multiplicity]

[length of the longest pair within the cluster]

[number of points in cluster]

[coordinates of 1st point] [number of possible species-2] [cluster function]

[coordinates of 2nd point] [number of possible species-2] [cluster function]

etc.

repeat,etc.

(Multiplicity and length are ignored when reading in the clusters.out file.)

For each ’point’ the following convention apply

-The coordinates are expressed in the coordinate system given in

the first line (or the first 3 lines) of the lat.in file.

-The ’number of possible species’ distinguishes between binaries,ternaries,etc...

Since each site can accomodate any number of atom types,

this is specified for each point of the cluster.

-In multicomponent system,the cluster function are numbered from 0 to number of possible species-2.

In the simple of a binary system [number of possible species-2] [cluster function] are just 0 0.

For a ternary,the possible values are 1 0 and 1 1.

All the utilities that are not yet multicomponent-ready just ignore the entries [number of possible species-2]

Convention used to calculate the correlations:

The cluster functions in a m-component system are defined as

function ’0’:-cos(2*PI* 1 *s/m)

function ’1’:-sin(2*PI* 1 *s/m)

.

.

.

-cos(2*PI*[m/2]*s/m)

-sin(2*PI*[m/2]*s/m) <--- the last sin( ) is omitted if m is even

where the occupation variable s can take any values in {0,...,m-1}

and [...] denotes the ’round down’ operation.

Note that,these functions reduce to the single function (-1)^s in the binary case.

38 CHAPTER 7.COMMAND REFERENCE

Special options:

-sym:Just find the space group and then abort.

-clus:Just find space group and clusters and then abort.

-z:To find symmetry operations,atoms are considered to lie on

top of one another when they are less than this much apart.

-sig:Number of significant digits printed.

->Cautions

When vacancies are specified,the program may not be able to warn

you that the structure and the lattice just don’t fit.

Carefully inspect the corrdump.log file!

If the structure has significant cell shape relaxations,the program

will be unable to find how it relates to the ideal lattice.

The problem gets worse as the supercell size of the structure gets

bigger.

There is no limit on how far an atom in a structure can be from

the ideal lattice site.The program first finds the atom that can

be the most unambiguously assigned to a lattice site.It then

finds the next best assignement and so on.This is actually a

pretty robust way to do this.But keep in mind that the -z option

does NOT control this process.

7.1.2 cv

Help for cv

Command-line options:

-g:Favor cluster choices where the ground state line is correct.

(It is suggested to turn this feature on if you have trouble getting the

right ground states).

-w:Weight structures by w/(struct_energy-gs_energy+w)

(recommended value:start with 1.and decrease down to about 0.010 (eV)

if you have trouble getting the correct ground states.

Default:all structure have equal weight)

-p:Penality for structures that lie below the ground state line.

(recommended value:start with 1.and increase up to about 20.

if you have trouble getting the correct ground states.

Default:0)

-> corr.in

table of correlations,one structure per line

(exactly the output of corrdump)

-> energy.in

column of energy values,one per line,in the same order as in the corr.in file.

If energy is unknown,put ’x’.

7.1.MAN PAGES 39

-> include.in

This file can be omitted.

It gives a list of clusters than must be part of the cluster expansion.

(Each number in this file indicates a column in the corr.in file.)

-> weight.in

This file can be omitted.

It indicates the weight that must be given to each structure.

Usually this file is copied from the weight_sug.out file obtained from a previous run.

Each weight in this file is multiplied by

gs_prec/(structure_energy-ground_state_energy+gs_prec)

(see above).

-> clusters.out

A list of the clusters (in the same format as generated by either maps

or corrdump)

OUTPUT FILES

-> fit.out

Contains the results of the fit,one structure per line and each line

has the following information:

concentration energy fitted_energy weight index

’concentration’ lies between 0 and 1.

’energy’ is the true formation energy.

’fitted_energy’ is the predicted formation energy.

’weight’ is the weight of this structure in the fit.

’index’ is the structure number (not counting structure of unknown energies)

-> predstr.out

Contains the predicted energy of all structures whose true energy is unknown.

Format:one structure per line,and each line has the following information:

concentration predicted_energy -1 status

the ’-1’ is for compatibility with maps.

status is ’u’ (for compatibility with maps) and a ’g’ is appended to status if

that structure is predicted to be a ground state.

To list all predicted ground states,type

grep ’g’ predstr.out

-> gs.out

The ground states,as determined by energies given in energy.in.

Each line is a concentration,energy pair.

-> gs_fitted.out

The ground states,as determined by energies predicted from

the cluster expansion.(Structures for which the true energy is

unknown are omitted.)

Each line is a concentration,energy pair.

40 CHAPTER 7.COMMAND REFERENCE

-> weight_sug.out

If the ground states are incorrectly predicted by the cluster expansion,

this file contains suggested weight that should correct the problem.

just type

cp weight_sug.out weight.in

and rerun the program.

-> weight_used.out

Weights actually used to do the fit.

-> fit.gnu

A gnuplot script that display all the relevant information.

Just type:

gnuplot fit.gnu

-> eci.out

The values of the fitted eci,in the same order as in the corr.in file.

7.1.3 emc2

Easy Monte Carlo Code (emc2)

by Axel van de Walle

Command line parameters:

-T0:initial temperature

-T1:final temperature

-dT:temperature step

-db:inverse temperature step

Temperatures are given in units of energy unless the -k option is set.

-dT and -db are mutually exclusive.Which option you use determines

whether T or 1/T are unformly spaced.The output file always shows T.

Avoid setting -T0 or -T1 to 0:The output will be nonsensical.

-k:Sets boltman’z constant (default k=1).This only affects how

temperatures are converted in energies.-k=8.617e-5 lets you enter

temperatures in kelvins when energies are in eV.

(You can also select this value by using the -keV option.)

-mu0:initial chemical potential

-mu1:final chemical potential

By default,these are input as dimensionless values defined as

follows:If x is integer,x is the chemical potential that

stabilizes a two phase equilibrium between ground state x-1 and

x.(Ground states are numbered starting at 0.) Fractional values

interpolate linearly between these integer values.Negative values

or values larger than the number of ground states - 1 are allowed.

7.1.MAN PAGES 41

The values of mu are found by linear extrapolation.If the -abs

option is specified,the value of mu are in units of energy per spin

value (as in the output file).(The ground states are read in from

the file gs_str.out.)

If there are only two ground states,the only correction performed is

to shift mu so that mu=0 stabilizes a two-phase equilibrium between

the two ground states.

If there are less than 2 ground states (!),no correction is made.

-dmu:chemical potential step (expressed in the same units as mu0 and mu1).

NOTE:If mu1 is omitted,only a scan through T is performed keeping mu=mu0.

If T1 is omitted,only scan through mu is performed keeping T=T0.

-gs:Gives the index of the ground state to use as an initial spin

configuration (the leftmost pure element is numbered 0).If the

index is -1,the disordered state with an average spin of zero

is used as the starting configuration.

-phi0:value of the grand canonical potential at the initial point of

the run.If left unspecified,it is set to the grand canonical

potential of given by either the 1-spin Low Temperature Expansion

or the High Temperature Expansion,depending whether the initial

state is an ordered or a disordered phase.

-er:enclosed radius.The Monte Carlo cell will the smallest possible

supercell of unit cell of the initial configuration such that a

sphere of that radius fits inside it.This allows you to specify

the system size in a structure-independent fashion.

-innerT:by default,the inner loop is over values mu while the outer

loop is over values of T.This flag permutes that order.

-eq:number of equilibration passes.(Equilibration is performed at

the beginning of each step of the outer loop.)

-n:number of Monte Carlo passes performed to evaluate thermodynamic

quanties at each step of the inner loop.

-dx:instead of specifying -eq and -n,you can ask the code to equilibrate

and run for a time such that the average concentration is accurate

within the target precision specifified by -dx=.

-tstat:Critical value of the test for discontinuity.The code is

able to catch phase transformations (most of the time) when

going from an ordered phase to another or to the disordered

state.This involves a statistical test which a

user-specified confidence level.The default,3,corresponds

to a 0.4% chance of finding a transition where there is

none.(Refer to a standard normal table.) -tstat=0 turns off

this option.Suggestion:if a phase transition is

undetected,first try to reduce dT or dmu or increase n or decrease dx

before toying around with this parameter.Also:beware of

42 CHAPTER 7.COMMAND REFERENCE

hysteresis.

-sigdig:Number of significant digits printed.Default is 6.

-o:Name of the output file (default:mc.out).

Tricks:

To read parameters from a file,use:

emc2 ‘cat inputfile‘

where inputfile contains the commands line options.

To selectively display a few of the output quantities,use:

emc2 [options] | cut -f n1,n2,n3,...

where n1,n2,n3,...are the column number desired (see below).

Input files:

lat.in:description of the lattice.

clusters.out:describes the clusters.

eci.out:provides the ECI.

gs_str.out:a list of ground states,in increasing order of concentration.

These 4 files can be created by maps.

See maps documentation (maps -h) for a description of the formats.

Optional input file:

teci.out:if present,provides temperature-dependent eci (overrides eci.out)

(Note that,even when the teci.out file is used,column 6 of the output file

reflects only the configurational contribution to the heat capacity.)

The format this file is:

[maximum temperature:Tm]

[number of temperatures where eci are provided:nT]

[ECIs for temperature 0]

[ECIs for temperature Tm/(nT-1)]

[ECIs for temperature 2*Tm/(nT-1)]

...

[ECIs for temperature Tm]

Note that these numbers can be seperated by blanks or newlines,as desired.

Format of the output file:

Each line contains,in order:

1) T:Temperature

2) mu:chemical potential (derivative of the free energy wrt to average spin)

3) E-mu*x:Average energy (per spin)

4) x:Average Concentration [ranges from -1 to 1]

5) phi:grand canonical potential

6) E2:Variance of the energy (proportional to heat capacity)

7) x2:Variance of the concentration (proportional to susceptibility)

7.1.MAN PAGES 43

8) E_lte-mu*x_lte:calculated with a one spin Low Temperature Expansion

9) x_lte

10) phi_lte

11) E_mf-mu*x_mf:calculated with the Mean Field approximation

12) x_mf

13) phi_mf

14) E_hte-mu*x_hte:calculated with a High Temperature Expansion (ideal solution + polynomial in x)

15) x_hte

16) phi_hte

17) lro:Long Range Order parameter of the initial ordered phase (=0 if initial phase is disordered).

18-) corr:the average correlations associated with each cluster.

NOTE:to obtain ’canonical’ rather than grand canonical quantities,

use the -g2c option.This has the effect of adding mu*x to columns

3,5,8,10,11,13,14,16.

7.1.4 felec

This code calculates the electronic free energy within the one-electron

and temperature-independent bands approximations.

It needs an dos.out input file (whose name can be changed with -dos option) that

has the following format:

[number of electron in unitcell]

[energy width of each bins used to calculate the dos]

[a multiplicative scale factor to adjust units]

[the density in each bin,in states/unit cell/energy] <- repeated

The code calculates the electronic free energy from temperature T0 to T1 in steps of dT.

a) The defaults are T0=0 T1=2000 dT=100.

b) If a file Trange.in exists in the upper directory,it is used to set T0,T1,dT:

Trange.in must contain two numbers on one line separated by a space:T1 (T1/dT+1).

## Comments 0

Log in to post a comment